Hot Rolling Cold Rolling
Definition: The process of plastically deforming metal
by passing it between rolls.
Most widely used, high production and close tolerance.
Friction between the rolls and the metal surface
produces high compressive stress.
Hot-working (unless mentioned cold rolling.)
In a rolling process, the state of stress of the
material undergoing deformation is
(a) pure compression
(b) pure shear
(c) compression and shear
(d) tension and shear
Done above the recrystallization temp.
Results fine grained structure.
Surface quality and final dimensions are less accurate.
Breakdown of ingots into blooms and billets is done by
hot-rolling. This is followed by further hot-rolling into
plate, sheet, rod, bar, pipe, rail.
Hot Rolling Video
Done below the recrystallization temp..
Products are sheet, strip, foil etc. with good surface
finish and increased mechanical strength with close
Performed on four-high or cluster-type rolling mills.
(Due to high force and power)
Cold Rolling and Grain
Ring rolls are used for tube rolling, ring rolling.
As the rolls squeeze and rotate, the wall thickness is
reduced and the diameter of the ring increases.
Shaped rolls can be used to produce a wide variety of
Ring rolls are made of spheroidized graphite bainitic and
pearlitic matrix or alloy cast steel base.
Ring Rolling Video
Ring rolling is used
(a) To decrease the thickness and increase
(b) To increase the thickness of a ring
(c) For producing a seamless tube
(d) For producing large cylinder
In sheet rolling we are only attempting to reduce the
cross section thickness of a material.
A continuous form of three-point bending is roll
bending, where plates, sheets, and rolled shapes can
be bent to a desired curvature on forming rolls.
Upper roll being adjustable to control the degree of
Roll Bending Video
IES – 2006
Which one of the following is a continuous bending
process in which opposing rolls are used to produce
long sections of formed shapes from coil or strip
(a) Stretch forming (b) Roll forming
(c) Roll bending (d) Spinning
Shape Rolling Video
Pack rolling involves hot rolling multiple sheets of
material at once, such as aluminium foil.
A thin surface oxide film prevents their welding.
Used to produce threads in substantial quantities.
This is a cold-forming process in which the threads are
formed by rolling a thread blank between hardened dies
that cause the metal to flow radially into the desired
No metal is removed, greater strength, smoother, harder,
and more wear-resistant surface than cut threads.
Thread rolling contd….
Major diameter is always greater than the diameter of the
Blank diameter is little larger than the pitch diameter of
Restricted to ductile materials.
Manufacture of gears by rolling
The straight and helical teeth of disc or rod type external
steel gears of small to medium diameter and module
are generated by cold rolling.
High accuracy and surface integrity.
Employed for high productivity and high quality. (costly
Larger size gears are formed by hot rolling and then
finished by machining. Fig. Production of teeth of spur gears by rolling
It is a variation of rolling called roll piercing.
The billet or round stock is rolled between two rolls,
both of them rotating in the same direction with their
axes at an angle of 4.5 to 6.5 degree.
These rolls have a central cylindrical portion with the
sides tapering slightly. There are two small side rolls,
which help in guiding the metal.
Because of the angle at which the roll meets the metal,
it gets in addition to a rotary motion, an additional
axial advance, which brings the metal into the rolls.
This cross-rolling action makes the metal friable at the
centre which is then easily pierced and given a
cylindrical shape by the central-piercing mandrel.
Use in high strength
material and cold
En sab tam jham sae
Buckling nhi hoti
Use for Supper alloy
and cold working
Advantage of small roller in 4-High
A small roll diameter is advantageous because less roll
is in contact with the material which results in a lower
FORCE and ENERGY requirement.
Let pressure required for final
For Fig A For Fig. B
Since roller size is
small, let it will be 5m2
Force reduce from
100N to 50N
Area involment is very-2 high in bigger roller compare
to smaller roller.
Power supply always given to working roller, back up
roller rolls due to Friction
Problem with small roller
Reduction of stiffness
using Back UP
Consist of a pair of heavy backing rolls surrounded by a large
number of planetary rolls.
Each planetary roll gives an almost constant reduction to the
slab as it sweeps out a circular path between the backing rolls
and the slab.
As each pair of planetary rolls ceases to have contact with the
work piece, another pair of rolls makes contact and repeat
The overall reduction is the summation of a series of small
reductions by each pair of rolls. Therefore, the planetary mill
can reduce a slab directly to strip in one pass through the
The operation requires feed rolls to introduce the slab into
the mill, and a pair of planishing rolls on the exit to improve
the surface finish.
The roll gap must be perfectly parallel to produce sheets/plates with
equal thickness at both ends
Camber can be used to correct the roll deflection (at only
one value of the roll force).
Lubrication for Rolling
Hot rolling of ferrous metals is done without a lubricant.
Hot rolling of non-ferrous metals a wide variety of
compounded oils, emulsions and fatty acids are used.
Cold rolling lubricants are water-soluble oils, low-
viscosity lubricants, such as mineral oils, emulsions,
paraffin and fatty acids.
Defects in Rolling
Defects What is Cause
impurities in the
Wavy edges Strip is thinner
along its edges
than at its centre.
Due to roll bending
edges elongates more
Alligatoring Edge breaks Non-uniform
GATE – 2009 (PI)
Anisotropy in rolled components is caused by
(a) changes in dimensions
(b) scale formation
(c) closure of defects
(d) grain orientation
Formula in Rolling
Geometry of Rolling Process
The largest angle that will just grip a lump between the
jaws, rolls, or mantle and ring of a crusher. Also know
n as angle of bite; nip.
Angle of nip = 2 α
Total reduction or “draft” taken in rolling.
Usually, the reduction in blooming mills is about 100
mm and in slabbing mills, about 50 to 60 mm.
Maximum Draft Possible
h=h -h =2(R-Rcos )=D(1-cos )
Numberof pass needed
Therefore Free engagement/for unaided
entery will occur when µ > tan α
o Generally rolling increases the
work width from an initial value
of bo to a final one of bf and this
is called spreading.
o The inlet and outlet volume
rates of material flow must be
the same, that is,
hobovo = hfbfvf
where vo and vf are the entering
and exiting velocities of the
A mild steel plate has to be rolled in one pass such that
the final plate thickness is 2/3rd of the initial thickness,
with the entrance speed of 10 m/min and roll diameter
of 500 mm. If the plate widens by 2% during rolling, the
exit velocity (in m/min) is …… ………
Torque and Power
Where λ is 0.5 for hot-rolling and 0.45 for cold-rolling.
The total rolling load is distributed
over the arc of contact in the typical
friction-hill pressure distribution.
However the total rolling load can be
assumed to be concentrated at a
point along the act of contact at a
distance a from the line of centres of
The ratio of the moment arm a to the
projected length of the act of contact
Lp can be given as
The torque MT is equal to the total rolling load P
multiplied by the effective moment arm a. Since there are
two work rolls, the torque
Projected length (Lp) = R sinα = √RΔh, mm
Projected Area(Ap)= Lp × b, mm2
Roll Separating Force (F )= σ0 × Lp × b, N
Armlength (a in mm)=0.5 × Lp for hot rolling
=0 45 × Lp for cold
Torque per roller (T )= F ×a/1000, Nm
Total power for two roller=2Tω, in W
In rolling a strip between two rolls, the position of
the neutral point in the arc of contact does not
Material of the rolls
While rolling a strip the peripheral velocity of
the roll is ….A…..than the entry velocity of the
strip and is ……B …..the exit velocity of the
(a) less than/greater less
(b) Greater than/less than
In a single pass rolling operation, a 20 mm thick
plate with plate width of 100 mm, is reduced to 18
mm. The roller radius is 250 mm and rotational
speed is 10 rpm. The average flow stress for the plate
material is 300 MPa. The power required for the
rolling operation in kW is closest to
The thickness of a metallic sheet is reduced from an
initial value of 16 mm to a final value of 10 mm in
one single pass rolling with a pair of cylindrical
rollers each of diameter of 400 mm. The bite angle
in degree will be
In a rolling process, sheet of 25 mm thickness is
rolled to 20 mm thickness. Roll is of diameter 600
mm and it rotates at 100 rpm. The roll strip contact
length will be
(a) 5 mm (b) 39 mm
(c) 78 mm (d) 120 mm
GATE – 2012 Same Q in GATE – 2012 (PI)
In a single pass rolling process using 410 mm
diameter steel rollers, a strip of width 140 mm and
thickness 8 mm undergoes 10% reduction of
thickness. The angle of bite in radians is
(a) 0.006 (b) 0.031
(c) 0.062 (d) 0.600
A 4 mm thick sheet is rolled with 300 mm diameter
rolls to reduce thickness without any change in its
width. The friction coefficient at the work-roll
interface is 0.1. The minimum possible thickness of
the sheet that can be produced in a single pass is
(a) 1.0 mm (b) 1.5 mm
(c) 2.5 mm (d) 3.7 mm
GATE – 2011 (PI)
The thickness of a plate is reduced from 30 mm to
10 mm by successive cold rolling passes using
identical rolls of diameter 600 mm. Assume that
there is no change in width. If the coefficient of
friction between the rolls and the work piece is 0.1,
the minimum number of passes required is
IES – 2001
A strip is to be rolled from a thickness of 30 mm to
15 mm using a two-high mill having rolls of
diameter 300 mm. The coefficient of friction for
unaided bite should nearly be
(a) 0.35 (b) 0.5
(c) 0.25 (d) 0.07
IES – 1993
In order to get uniform thickness of the plate by
rolling process, one provides
(a) Camber on the rolls
(b) Offset on the rolls
(c) Hardening of the rolls
(d) Antifriction bearings
IES – 1993
The blank diameter used in thread rolling will be
(a) Equal to minor diameter of the thread
(b) Equal to pitch diameter of the thread
(c) A little large than the minor diameter of the thread
(d) A little larger than the pitch diameter of the thread
IES – 1992
Thread rolling is restricted to
(a) Ferrous materials
(b) Ductile materials
(c) Hard materials
(d) None of the above
IAS – 2001
Consider the following characteristics of rolling
1. Shows work hardening effect
2. Surface finish is not good
3. Heavy reduction in areas can be obtained
Which of these characteristics are associated with hot
(a) 1 and 2 (b) 1 and 3
(c) 2 and 3 (d) 1, 2 and 3
IAS – 2000
Rolling very thin strips of mild steel requires
(a) Large diameter rolls
(b) Small diameter rolls
(c) High speed rolling
(d) Rolling without a lubricant
IAS – 2003
In one setting of rolls in a 3-high rolling mill, one
(a) One reduction in thickness
(b) Two reductions in thickness
(c) Three reductions in thickness
(d) Two or three reductions in thickness depending
upon the setting
IAS – 2007
Consider the following statements:
Roll forces in rolling can be reduced by
1. Reducing friction
2. Using large diameter rolls to increase the contact
3. Taking smaller reductions per pass to reduce the
Which of the statements given above are correct?
(a) 1 and 2 only (b) 2 and 3 only
(c) 1 and 3 only (d) 1, 2 and 3
The maximum possible draft in cold rolling of sheet
increases with the
(a) increase in coefficient of friction
(b) decrease in coefficient of friction
(c) decrease in roll radius
(d) increase in roll velocity